General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.85 g/cm³ Show Material materials with Density of 7.85 g/cm³ |

50.0 °C | 7.84 g/cm³ Show Material materials with Density of 7.84 g/cm³ | |

100.0 °C | 7.83 g/cm³ Show Material materials with Density of 7.83 g/cm³ | |

150.0 °C | 7.81 g/cm³ Show Material materials with Density of 7.81 g/cm³ | |

200.0 °C | 7.79 g/cm³ Show Material materials with Density of 7.79 g/cm³ | |

250.0 °C | 7.78 g/cm³ Show Material materials with Density of 7.78 g/cm³ | |

300.0 °C | 7.76 g/cm³ Show Material materials with Density of 7.76 g/cm³ | |

350.0 °C | 7.74 g/cm³ Show Material materials with Density of 7.74 g/cm³ | |

400.0 °C | 7.72 g/cm³ Show Material materials with Density of 7.72 g/cm³ | |

450.0 °C | 7.7 g/cm³ Show Material materials with Density of 7.7 g/cm³ | |

500.0 °C | 7.68 g/cm³ Show Material materials with Density of 7.68 g/cm³ | |

550.0 °C | 7.66 g/cm³ Show Material materials with Density of 7.66 g/cm³ | |

600.0 °C | 7.64 g/cm³ Show Material materials with Density of 7.64 g/cm³ | |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa |

20.0 °C | 211.31 - 212 GPa Show Material materials with Elastic modulus of 211.31 - 212 GPa | |

50.0 °C | 209.84 GPa Show Material materials with Elastic modulus of 209.84 GPa | |

100.0 °C | 206.79 - 207 GPa Show Material materials with Elastic modulus of 206.79 - 207 GPa | |

150.0 °C | 203.36 GPa Show Material materials with Elastic modulus of 203.36 GPa | |

200.0 °C | 199 - 200 GPa Show Material materials with Elastic modulus of 199 - 200 GPa | |

250.0 °C | 195.42 GPa Show Material materials with Elastic modulus of 195.42 GPa | |

300.0 °C | 191.49 - 192 GPa Show Material materials with Elastic modulus of 191.49 - 192 GPa | |

350.0 °C | 187.47 GPa Show Material materials with Elastic modulus of 187.47 GPa | |

400.0 °C | 183 - 184 GPa Show Material materials with Elastic modulus of 183 - 184 GPa | |

450.0 °C | 179.03 GPa Show Material materials with Elastic modulus of 179.03 GPa | |

500.0 °C | 174.72 - 175 GPa Show Material materials with Elastic modulus of 174.72 - 175 GPa | |

550.0 °C | 170.2 GPa Show Material materials with Elastic modulus of 170.2 GPa | |

600.0 °C | 164 - 166 GPa Show Material materials with Elastic modulus of 164 - 166 GPa | |

Unlock all property charts | ||

Elongation | 20.0 °C | 21 % Show Material materials with Elongation of 21 % |

Elongation, transverse | 20.0 °C | 19 % Show Material materials with Elongation, transverse of 19 % |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

50.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

100.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

150.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

200.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

250.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

300.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

350.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

400.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

450.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

500.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

550.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

600.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 82.31 GPa Show Material materials with Shear modulus of 82.31 GPa |

50.0 °C | 81.62 GPa Show Material materials with Shear modulus of 81.62 GPa | |

100.0 °C | 80.34 GPa Show Material materials with Shear modulus of 80.34 GPa | |

150.0 °C | 78.97 GPa Show Material materials with Shear modulus of 78.97 GPa | |

200.0 °C | 77.4 GPa Show Material materials with Shear modulus of 77.4 GPa | |

250.0 °C | 75.83 GPa Show Material materials with Shear modulus of 75.83 GPa | |

300.0 °C | 74.16 GPa Show Material materials with Shear modulus of 74.16 GPa | |

350.0 °C | 72.5 GPa Show Material materials with Shear modulus of 72.5 GPa | |

400.0 °C | 70.73 GPa Show Material materials with Shear modulus of 70.73 GPa | |

450.0 °C | 69.06 GPa Show Material materials with Shear modulus of 69.06 GPa | |

500.0 °C | 67.3 GPa Show Material materials with Shear modulus of 67.3 GPa | |

550.0 °C | 65.53 GPa Show Material materials with Shear modulus of 65.53 GPa | |

600.0 °C | 63.67 GPa Show Material materials with Shear modulus of 63.67 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 410 - 530 MPa Show Material materials with Tensile strength of 410 - 530 MPa |

Yield strength Rp0.2 | 20.0 °C | 235 - 255 MPa Show Material materials with Yield strength Rp0.2 of 235 - 255 MPa |

200.0 °C | 190 - 205 MPa Show Material materials with Yield strength Rp0.2 of 190 - 205 MPa | |

250.0 °C | 170 - 185 MPa Show Material materials with Yield strength Rp0.2 of 170 - 185 MPa | |

300.0 °C | 150 - 160 MPa Show Material materials with Yield strength Rp0.2 of 150 - 160 MPa | |

350.0 °C | 135 - 140 MPa Show Material materials with Yield strength Rp0.2 of 135 - 140 MPa | |

400.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | |

450.0 °C | 125 MPa Show Material materials with Yield strength Rp0.2 of 125 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | |

20.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

100.0 °C | 1.22E-5 - 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.22E-5 - 1.25E-5 1/K | ||

200.0 °C | 1.29E-5 - 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.29E-5 - 1.3E-5 1/K | ||

300.0 °C | 1.34E-5 - 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.34E-5 - 1.36E-5 1/K | ||

400.0 °C | 1.4E-5 - 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.4E-5 - 1.41E-5 1/K | ||

500.0 °C | 1.43E-5 - 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.43E-5 - 1.45E-5 1/K | ||

600.0 °C | 1.46E-5 - 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.46E-5 - 1.49E-5 1/K | ||

Unlock all property charts | |||

Max service temperature | 500 °C Show Material materials with Max service temperature of 500 °C | Typical for Carbon Steel | |

Max service temperature, long | 0 - 500 °C Show Material materials with Max service temperature, long of 0 - 500 °C | ||

Melting point | 1480 - 1526 °C Show Material materials with Melting point of 1480 - 1526 °C | Typical for Low Carbon Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | ||

100.0 °C | 479 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 479 - 500 J/(kg·K) | ||

200.0 °C | 499 - 540 J/(kg·K) Show Material materials with Specific heat capacity of 499 - 540 J/(kg·K) | ||

300.0 °C | 517 - 580 J/(kg·K) Show Material materials with Specific heat capacity of 517 - 580 J/(kg·K) | ||

400.0 °C | 536 - 620 J/(kg·K) Show Material materials with Specific heat capacity of 536 - 620 J/(kg·K) | ||

500.0 °C | 558 - 690 J/(kg·K) Show Material materials with Specific heat capacity of 558 - 690 J/(kg·K) | ||

600.0 °C | 587 - 780 J/(kg·K) Show Material materials with Specific heat capacity of 587 - 780 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 53.4 W/(m·K) Show Material materials with Thermal conductivity of 53.4 W/(m·K) | |

100.0 °C | 52.9 - 53 W/(m·K) Show Material materials with Thermal conductivity of 52.9 - 53 W/(m·K) | ||

200.0 °C | 50 - 50.3 W/(m·K) Show Material materials with Thermal conductivity of 50 - 50.3 W/(m·K) | ||

300.0 °C | 46.7 - 47 W/(m·K) Show Material materials with Thermal conductivity of 46.7 - 47 W/(m·K) | ||

400.0 °C | 43 - 43.3 W/(m·K) Show Material materials with Thermal conductivity of 43 - 43.3 W/(m·K) | ||

500.0 °C | 39.8 - 40 W/(m·K) Show Material materials with Thermal conductivity of 39.8 - 40 W/(m·K) | ||

600.0 °C | 36 - 36.7 W/(m·K) Show Material materials with Thermal conductivity of 36 - 36.7 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 14.8 mm²/s Show Material materials with Thermal diffusivity of 14.8 mm²/s | |

100.0 °C | 13.6 mm²/s Show Material materials with Thermal diffusivity of 13.6 mm²/s | ||

200.0 °C | 12.1 mm²/s Show Material materials with Thermal diffusivity of 12.1 mm²/s | ||

300.0 °C | 10.6 mm²/s Show Material materials with Thermal diffusivity of 10.6 mm²/s | ||

400.0 °C | 9.2 mm²/s Show Material materials with Thermal diffusivity of 9.2 mm²/s | ||

500.0 °C | 7.7 mm²/s Show Material materials with Thermal diffusivity of 7.7 mm²/s | ||

600.0 °C | 6.2 mm²/s Show Material materials with Thermal diffusivity of 6.2 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.95E-7 Ω·m Show Material materials with Electrical resistivity of 1.95E-7 Ω·m |

50.0 °C | 2.11E-7 Ω·m Show Material materials with Electrical resistivity of 2.11E-7 Ω·m | |

100.0 °C | 2.3E-7 - 2.42E-7 Ω·m Show Material materials with Electrical resistivity of 2.3E-7 - 2.42E-7 Ω·m | |

150.0 °C | 2.76E-7 Ω·m Show Material materials with Electrical resistivity of 2.76E-7 Ω·m | |

200.0 °C | 3E-7 - 3.14E-7 Ω·m Show Material materials with Electrical resistivity of 3E-7 - 3.14E-7 Ω·m | |

250.0 °C | 3.55E-7 Ω·m Show Material materials with Electrical resistivity of 3.55E-7 Ω·m | |

300.0 °C | 3.8E-7 - 4.02E-7 Ω·m Show Material materials with Electrical resistivity of 3.8E-7 - 4.02E-7 Ω·m | |

350.0 °C | 4.49E-7 Ω·m Show Material materials with Electrical resistivity of 4.49E-7 Ω·m | |

400.0 °C | 4.8E-7 - 5.02E-7 Ω·m Show Material materials with Electrical resistivity of 4.8E-7 - 5.02E-7 Ω·m | |

450.0 °C | 5.59E-7 Ω·m Show Material materials with Electrical resistivity of 5.59E-7 Ω·m | |

500.0 °C | 6E-7 - 6.21E-7 Ω·m Show Material materials with Electrical resistivity of 6E-7 - 6.21E-7 Ω·m | |

550.0 °C | 6.83E-7 Ω·m Show Material materials with Electrical resistivity of 6.83E-7 Ω·m | |

600.0 °C | 7.4E-7 - 7.55E-7 Ω·m Show Material materials with Electrical resistivity of 7.4E-7 - 7.55E-7 Ω·m | |

Unlock all property charts |

Magnetic

Property | Value | Comment |
---|---|---|

Curie temperature | 770 °C Show Material materials with Curie temperature of 770 °C | Typical for Low Carbon Steel |

Chemical properties

Property | Value |
---|---|

Carbon | 0.21 % Show Material materials with Carbon of 0.21 % |

Manganese | 0.4 - 1.2 % Show Material materials with Manganese of 0.4 - 1.2 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.1 - 0.35 % Show Material materials with Silicon of 0.1 - 0.35 % |

Sulfur | 0.04 % Show Material materials with Sulfur of 0.04 % |